Cryogenic transmission electron microscopy: the technique of choice for the characterization of polymeric nanocarriers
© The Author(s). 2017
Received: 1 May 2017
Accepted: 8 May 2017
Published: 22 May 2017
This letter is meant to make scientists aware of the proper application of transmission electron microscopy (TEM) for the assessment of polymeric self-assemblies. Cryogenic (cryo)-TEM should be the method of choice. Here, we show the difference in morphologies observed in the same sample when using cryo-TEM and when using TEM with drying, demonstrating the importance of choosing the proper method.
In our article published on February 2016, we have reported a method for radiolabeling polystyrene-b-poly(ethylene oxide) (PS-b-PEO) diblock copolymer micelles . As part of the physical characterization of the produced nanocarriers, we have done analysis with transmission electron microscopy (TEM) using the drying method. However, it was brought to our attention that this characterization method involving drying is not ideal for the investigation of the morphologies of self-assemblies, even when these assemblies are composed of block copolymers having extremely slow-exchange kinetics. Cryo-TEM is the technique that should be used for the assessment of soft-matter assemblies, as pointed out in the critical study carried out by Stuart et al. . The major cause of discrepancies between the drying method and cryo-TEM is related to the preparation procedure of the samples on the TEM grid. With the drying method, a drop of the sample is dried onto a grid by evaporation of the solvent from the sample, which can result in deformation or even complete destruction of the particles. In the case of cryo-TEM, the sample is rapidly frozen on the grid, i.e., instantly vitrified, impairing any changes of the morphology of the particles [2–5].
In regard to our previous publication , this means that the size range of the nano-assemblies is somewhat different from what we have reported based on the TEM analysis. On the other hand, the results obtained by dynamic light scattering, as reported, do give a good indication on the actual size range and polydispersity of the self-assemblies. We believe that our new findings do not affect the conclusions on the radiolabeling of the polymeric carriers, as this mechanism remains unchanged. This mechanism is based on the loading of the radionuclide in the hydrophobic compartment of the nanocarriers by employing a lipophilic ligand to complex the metal. In the case of the micelles, the PS core was radiolabelled, and in the case of the vesicles, the hydrophobic part of the bi-layered membrane was used to retain the radiolabel.
With this letter, we would like to emphasize that with the more suitable technique, cryo-TEM, we were able to get better understanding on our method and the produced self-assemblies. Furthermore, with this letter, we hope to help other researchers to realize that TEM using the drying method as well as scanning electron microscopy or atomic force microscopy are not appropriate techniques for determining the morphology of any soft-matter species [2–4].
Materials and methods
For preparation of the samples: in a 20 mL glass vial, 100 μL of a solution of PS-b-PEO 9500-18000 block copolymer in chloroform was added to 2.3 mL of 10 mM HEPES buffer pH 7.4 to reach the final polymer concentration of 10 mg/mL. The mixture was stirred at room temperature in a fume hood using a glass stirring bar in a vial without cap for about 2 h until the chloroform had evaporated.
The JEOL JEM-1400Plus, 120 kV transmission electron microscope with a LaB6 emitter, was used for the analysis.
For the drying method: directly before analysis, 5 μL of sample was put onto a hydrophilized TEM grid (Quantifoil “R1.2/1.3” holey carbon film on Cu 200 mesh), the excess of the sample was removed with filter paper, and the grid was left to dry for about 1 min before placing the grid, using a sample holder, in the microscope for TEM analysis.
For cryo-TEM, the Leica EM GP automatic plunge freezer was used to prepare the sample on the TEM grid. The blotting chamber was kept at 20 °C and >90% RH, 5 μL of sample was put onto the hydrophilized grid, and the grid was blotted (one-sided front side blotting) with filter paper for 4 s before plunging in liquid ethane. The grid was transferred to the cryo sample holder and inserted in the microscope.
AL performed the sample analysis. AL and AD wrote the manuscript. Both authors read and approved the final manuscript.
The authors declare to have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Open AccessThis article is distributed under the terms of the Creative Commons Attribution 4.0 International License (http://creativecommons.org/licenses/by/4.0/), which permits unrestricted use, distribution, and reproduction in any medium, provided you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made.
- Laan AC, Santini C, Jennings L, de Jong M, Bernsen MR, Denkova AG. Radiolabeling polymeric micelles for in vivo evaluation: a novel, fast, and facile method. EJNMMI Res. 2016;6:12.View ArticlePubMedPubMed CentralGoogle Scholar
- Franken LE, Boekema EJ, Stuart MCA: Transmission electron microscopy as a tool for the characterization of soft materials: application and interpretation. Adv Sci. 2017: 1600476Google Scholar
- Patterson JP, Robin MP, Chassenieux C, Colombanib O, O’Reilly RK. The analysis of solution self-assembled polymeric nanomaterials. Chem Soc Rev. 2014;43:2412–25.View ArticlePubMedGoogle Scholar
- Friedrich H, Frederik PM, de With G, Sommerdijk NAJM. Imaging of self-assembled structures: interpretation of TEM and cryo-TEM images. Angew Chem Int Ed. 2010;49:7850–8.View ArticleGoogle Scholar
- Cui H, Hodgdon TK, Kaler EW, Abezgauz L, Danino D, Lubovsky M, Talmond Y, Pochan DJ. Elucidating the assembled structure of amphiphiles in solution via cryogenic transmission electron microscopy. Soft Matter. 2007;3:945–55.View ArticleGoogle Scholar